- Home
- Documents
*SUPPLEMENTARY INFORMATION Two distinct ... SUPPLEMENTARY INFORMATION Two distinct mechanisms upon...*

prev

next

out of 2

View

0Download

0

Embed Size (px)

SUPPLEMENTARY INFORMATION

Two distinct mechanisms upon absorption of volatile organic compounds into Siloxane Polymers John Saunders, Hao Chen, Chris Brauer, McGregor Clayton, and Hans-Peter Loock*

Department of Chemistry Queen’s University Kingston, ON, K7L 3N6, Canada

hploock@chem.queensu.ca

Fit of the absorption and desorption curves The manuscript describes the fit of the absorption and desorption curves to equations that describe the diffusion of the gases into siloxane polymers. Equation (4) of the main manuscript can be written as

\* MERGEFORMAT S(1)

2 2 0 2 2 2

1 0

2 18 11 exp 42 1

K i

iabsorption i n

n D t t X t X

dn

And the corresponding desorption curve is

\* MERGEFORMAT S(2)

2 2 0 0 2 2 2

1 0

2 18 1 exp 42 1

K i

idesorption i n

n D t t X t X

dn

In the manuscript it is argued that a biexponential fit (K=2) is adequate for most curves and accordingly two diffusion constants Di are given for each process, i.e. for absorption and desorption. While the quality of the residuals provides a good indicator for the adequacy of the fit, a more careful analysis is required to ensure that the data are neither “overfitted” nor “underfitted”. Figure S1 shows the absorption and desorption curve following exposure of a PDMS film to 200 Pa m-xylene and nitrogen. The three functions with K=1 (blue), K=2 (red) and K=3 (green) all provide excellent fits with a correlation coefficient R2> 0.98. The fit and residuals for the K=2 and 3 are nearly identical, indicating that fitting the data to three distinct rates is not improving the fit quality over the b-exponential model.

The adequacy of the bi-exponential fit is further supported by the analysis of the co-variance matrix. Table S1 lists the results from the fit using the Levenberg-Marquardt algorithm (implemented through Microcal Origin 6.0). The uncertainties are determined in this algorithm from the covariance matrix and clearly indicate that a third exponential function overfits the data. The fit also indicates that two exponential functions give only a modest improvement of the coefficient of determination compared to fits with a single exponential function. We nevertheless believe that a second term improves the fit quality, because both of the two additional fit parameters may be obtained with low uncertainties, i.e. their covariance terms are low. A similar analysis was carried out for absorption and desorption curves of the other analytes, except where indicated in the text. Note that the uncertainties given in Table 3 of the main text arise from the distribution of values obtained in at least five different absorption and desorption experiments. The reproducibility of the kinetics between runs gave uncertainties of several 10%, which is much larger than the uncertainties arising from the fits to each of the curves.

Electronic Supplementary Material (ESI) for Soft Matter. This journal is © The Royal Society of Chemistry 2018

0 500 1000 1500 2000 2500 3000 3500

0.00

0.01

0.02 m

-x yle

ne c

on ce

nt ra

tio n,

X

0 500 1000 1500 2000 2500 3000 3500 -0.003

-0.002

-0.001

0.000

0.001

0.002

0.003

0.004

1-exp 2-exp 3-exp

Rr es

id ua

l

Time / s Figure S1: Absorption and desorption of m-xylene at 200 Pa into a PDMS polymer film akin to Fig 4 of the main text. The fits to K = 1, 2 and 3 independent diffusion processes according to equations \* MERGEFORMAT S(1) and \* MERGEFORMAT S(2) are given in blue, red and green respectively.

Table S1: Fit parameters of equations \* MERGEFORMAT S(1) and \* MERGEFORMAT S(2). and associated uncertainties obtained using a Levenberg-Marquardt fit to the data in Fig S1

Absorption Value (K=3) uncertainty Value (K=2) uncertainty Value (K=1) uncertainty X1 0.00597 73% 0.00785 2% 0.01714 0.12% X2 0.00654 14% 0.01013 1% 0 X3 0.00593 76% 0 0 D1 1.05 59% 4.453 4% 1.18991 0.80% D2 5.34 12% 0.569 3% D3 0.336 82% t0 680.9855 0.06% 678.9988 0% 663.245 0.09% R2 0.9974 0.9975 0.9942 Desorption X01 0.00874 5% 0.00863 2% 0.01736 0.35% X02 0.00724 12673% 0.0085 2% 0 X03 0.00128 71663% 0 0 D1 15.02 14% 17.91873 12% 2.48851 1.24% D2 1.38 696% 1.4331 3% D3 1.54 3941% t0 2391.961 0.08% 2395.802 0.03% 2375.659 0.03% R2 0.990 0.989 0.983